General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 8.4 g/cm³ Show Material materials with Density of 8.4 g/cm³ |

Mechanical

Property | Temperature | Value |
---|---|---|

Elastic modulus | 20.0 °C | 214 GPa Show Material materials with Elastic modulus of 214 GPa |

100.0 °C | 209 GPa Show Material materials with Elastic modulus of 209 GPa | |

200.0 °C | 205 GPa Show Material materials with Elastic modulus of 205 GPa | |

300.0 °C | 200 GPa Show Material materials with Elastic modulus of 200 GPa | |

400.0 °C | 194 GPa Show Material materials with Elastic modulus of 194 GPa | |

500.0 °C | 187 GPa Show Material materials with Elastic modulus of 187 GPa | |

600.0 °C | 180 GPa Show Material materials with Elastic modulus of 180 GPa | |

700.0 °C | 172 GPa Show Material materials with Elastic modulus of 172 GPa | |

800.0 °C | 163 GPa Show Material materials with Elastic modulus of 163 GPa | |

900.0 °C | 153 GPa Show Material materials with Elastic modulus of 153 GPa | |

1000.0 °C | 143 GPa Show Material materials with Elastic modulus of 143 GPa | |

Elongation | 20.0 °C | 30 % Show Material materials with Elongation of 30 % |

Elongation A80 | 20.0 °C | 30 % Show Material materials with Elongation A80 of 30 % |

Hardness, Brinell | 20.0 °C | 200 [-] Show Material materials with Hardness, Brinell of 200 [-] |

Tensile strength | 20.0 °C | 500 - 850 MPa Show Material materials with Tensile strength of 500 - 850 MPa |

Yield strength Rp0.2 | 20.0 °C | 240 MPa Show Material materials with Yield strength Rp0.2 of 240 MPa |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | 100.0 °C | 1.37E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.37E-5 1/K | |

200.0 °C | 1.39E-5 - 1.41E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.39E-5 - 1.41E-5 1/K | ||

300.0 °C | 1.44E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.44E-5 1/K | ||

400.0 °C | 1.45E-5 - 1.48E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.45E-5 - 1.48E-5 1/K | ||

500.0 °C | 1.51E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.51E-5 1/K | ||

600.0 °C | 1.53E-5 - 1.54E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.53E-5 - 1.54E-5 1/K | ||

700.0 °C | 1.58E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.58E-5 1/K | ||

800.0 °C | 1.61E-5 - 1.62E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.61E-5 - 1.62E-5 1/K | ||

900.0 °C | 1.64E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.64E-5 1/K | ||

1000.0 °C | 1.68E-5 - 1.69E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.68E-5 - 1.69E-5 1/K | ||

Unlock all property charts | |||

Max service temperature, long | 0 - 1150 °C Show Material materials with Max service temperature, long of 0 - 1150 °C | ||

Melting point | 1200 - 1480 °C Show Material materials with Melting point of 1200 - 1480 °C | Typical for Nickel Chromium Iron Alloy | |

Specific heat capacity | 20.0 °C | 455 - 460 J/(kg·K) Show Material materials with Specific heat capacity of 455 - 460 J/(kg·K) | |

100.0 °C | 475 J/(kg·K) Show Material materials with Specific heat capacity of 475 J/(kg·K) | ||

200.0 °C | 495 J/(kg·K) Show Material materials with Specific heat capacity of 495 J/(kg·K) | ||

300.0 °C | 508 J/(kg·K) Show Material materials with Specific heat capacity of 508 J/(kg·K) | ||

400.0 °C | 525 J/(kg·K) Show Material materials with Specific heat capacity of 525 J/(kg·K) | ||

500.0 °C | 550 J/(kg·K) Show Material materials with Specific heat capacity of 550 J/(kg·K) | ||

600.0 °C | 572 J/(kg·K) Show Material materials with Specific heat capacity of 572 J/(kg·K) | ||

700.0 °C | 602 J/(kg·K) Show Material materials with Specific heat capacity of 602 J/(kg·K) | ||

800.0 °C | 620 J/(kg·K) Show Material materials with Specific heat capacity of 620 J/(kg·K) | ||

900.0 °C | 630 J/(kg·K) Show Material materials with Specific heat capacity of 630 J/(kg·K) | ||

1000.0 °C | 635 J/(kg·K) Show Material materials with Specific heat capacity of 635 J/(kg·K) | ||

Unlock all property charts | |||

Thermal conductivity | 20.0 °C | 14.8 - 15 W/(m·K) Show Material materials with Thermal conductivity of 14.8 - 15 W/(m·K) | |

100.0 °C | 15.8 W/(m·K) Show Material materials with Thermal conductivity of 15.8 W/(m·K) | ||

200.0 °C | 17 W/(m·K) Show Material materials with Thermal conductivity of 17 W/(m·K) | ||

300.0 °C | 18.4 W/(m·K) Show Material materials with Thermal conductivity of 18.4 W/(m·K) | ||

400.0 °C | 20 W/(m·K) Show Material materials with Thermal conductivity of 20 W/(m·K) | ||

500.0 °C | 22 W/(m·K) Show Material materials with Thermal conductivity of 22 W/(m·K) | ||

600.0 °C | 24 W/(m·K) Show Material materials with Thermal conductivity of 24 W/(m·K) | ||

700.0 °C | 25.7 W/(m·K) Show Material materials with Thermal conductivity of 25.7 W/(m·K) | ||

800.0 °C | 27.5 W/(m·K) Show Material materials with Thermal conductivity of 27.5 W/(m·K) | ||

900.0 °C | 29.4 W/(m·K) Show Material materials with Thermal conductivity of 29.4 W/(m·K) | ||

1000.0 °C | 31.2 W/(m·K) Show Material materials with Thermal conductivity of 31.2 W/(m·K) | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | 20.0 °C | 1.03E-6 Ω·m Show Material materials with Electrical resistivity of 1.03E-6 Ω·m |

100.0 °C | 1.04E-6 Ω·m Show Material materials with Electrical resistivity of 1.04E-6 Ω·m | |

200.0 °C | 1.06E-6 Ω·m Show Material materials with Electrical resistivity of 1.06E-6 Ω·m | |

300.0 °C | 1.07E-6 Ω·m Show Material materials with Electrical resistivity of 1.07E-6 Ω·m | |

400.0 °C | 1.08E-6 Ω·m Show Material materials with Electrical resistivity of 1.08E-6 Ω·m | |

500.0 °C | 1.11E-6 Ω·m Show Material materials with Electrical resistivity of 1.11E-6 Ω·m | |

600.0 °C | 1.12E-6 Ω·m Show Material materials with Electrical resistivity of 1.12E-6 Ω·m | |

700.0 °C | 1.12E-6 Ω·m Show Material materials with Electrical resistivity of 1.12E-6 Ω·m | |

800.0 °C | 1.12E-6 Ω·m Show Material materials with Electrical resistivity of 1.12E-6 Ω·m | |

900.0 °C | 1.13E-6 Ω·m Show Material materials with Electrical resistivity of 1.13E-6 Ω·m | |

1000.0 °C | 1.14E-6 Ω·m Show Material materials with Electrical resistivity of 1.14E-6 Ω·m | |

Unlock all property charts |

Chemical properties

Property | Value |
---|---|

Aluminium | 0.3 % Show Material materials with Aluminium of 0.3 % |

Carbon | 0.05 - 0.1 % Show Material materials with Carbon of 0.05 - 0.1 % |

Chromium | 14 - 17 % Show Material materials with Chromium of 14 - 17 % |

Copper | 0.5 % Show Material materials with Copper of 0.5 % |

Iron | 6 - 10 % Show Material materials with Iron of 6 - 10 % |

Manganese | 1 % Show Material materials with Manganese of 1 % |

Nickel | 72 % Show Material materials with Nickel of 72 % |

Phosphorus | 0.02 % Show Material materials with Phosphorus of 0.02 % |

Silicon | 0.5 % Show Material materials with Silicon of 0.5 % |

Sulfur | 0.015 % Show Material materials with Sulfur of 0.015 % |

Titanium | 0.3 % Show Material materials with Titanium of 0.3 % |